#------------------------------------------------------------------------------
#$Date: 2015-06-04 13:53:05 +0300 (Thu, 04 Jun 2015) $
#$Revision: 137918 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/31/4343161.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4343161
loop_
_publ_author_name
'Artini, Cristina'
'Pani, Marcella'
'Carnasciali, Maria Maddalena'
'Buscaglia, Maria Teresa'
'Plaisier, Jasper Rikkert'
'Costa, Giorgio Andrea'
_publ_section_title
;
 Structural Features of Sm- and Gd-Doped Ceria Studied by Synchrotron
 X-ray Diffraction and μ-Raman Spectroscopy.
;
_journal_issue                   8
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4126
_journal_page_last               4137
_journal_paper_doi               10.1021/acs.inorgchem.5b00395
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'Ce O2'
_chemical_formula_weight         172.12
_chemical_name_common            'Cerium dioxide'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90.00000
_cell_angle_beta                 90.00000
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   5.40972(11)
_cell_length_b                   5.40972(11)
_cell_length_c                   5.40972(11)
_cell_measurement_temperature    295
_cell_volume                     158.316(6)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      295
_diffrn_detector                 'fast scintillator detector'
_diffrn_measurement_device_type  'Huber 4-axes X-ray diffractometer'
_diffrn_measurement_method       '2θ in the range 5-60 deg'
_diffrn_radiation_wavelength     0.749230
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    37.66
_exptl_absorpt_correction_type   none
_pd_char_colour                  'pale yellow'
_pd_instr_location
; powder diffraction beamline (MCX) of the Elettra synchrotron radiation
 facility located in Trieste, Italy
;
_pd_meas_2theta_range_inc        0.010003
_pd_meas_2theta_range_max        60.00000
_pd_meas_2theta_range_min        9.00000
_pd_meas_number_of_points        5101
_pd_meas_scan_method             step
_pd_prep_pressure                101
_pd_prep_temperature             1473
_pd_proc_2theta_range_inc        0.010003
_pd_proc_2theta_range_max        60.0150
_pd_proc_2theta_range_min        9.0150
_pd_proc_ls_background_function
;
linear interpolation between a set of background points with refinable heights
;
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_prof_R_factor        9.8210
_pd_proc_ls_prof_wR_expected     10.2454
_pd_proc_ls_prof_wR_factor       13.2573
_pd_proc_wavelength              0.749230
_pd_spec_mounting
' quartz capillary tube with inner diameter of 0.5 mm '
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              20
_pd_spec_size_equat              0.5
_refine_ls_goodness_of_fit_all   1.29
_refine_ls_number_parameters     80
_refine_ls_number_reflns         22
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            2.7157
_refine_ls_shift/su_max          0.1
_cod_data_source_file            ic5b00395_si_002.cif
_cod_data_source_block           CeO2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Cubic' changed to 'cubic' according
to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 
;
_cod_original_cell_volume        158.316(5)
_cod_database_code               4343161
_pd_proc_ls_prof_cr_factor       24.1235
_pd_proc_ls_prof_cwr_factor      22.6107
_pd_proc_ls_prof_cwr_expected    17.4738
_pd_proc_ls_prof_chi2            1.6744
_pd_proc_ls_prof_echi2           1.7619
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
x,-y,-z
-x,y,-z
-x,-y,z
y,z,x
-y,-z,x
y,-z,-x
-y,z,-x
z,x,y
-z,x,-y
-z,-x,y
z,-x,-y
y,x,z
-y,x,-z
y,-x,-z
-y,-x,z
z,y,x
-z,-y,x
-z,y,-x
z,-y,-x
x,z,y
x,-z,-y
-x,-z,y
-x,z,-y
-x,-y,-z
-x,y,z
x,-y,z
x,y,-z
-y,-z,-x
y,z,-x
-y,z,x
y,-z,x
-z,-x,-y
z,-x,y
z,x,-y
-z,x,y
-y,-x,-z
y,-x,z
-y,x,z
y,x,-z
-z,-y,-x
z,y,-x
z,-y,x
-z,y,x
-x,-z,-y
-x,z,y
x,z,-y
x,-z,y
x+1/2,y+1/2,z
x+1/2,-y+1/2,-z
-x+1/2,y+1/2,-z
-x+1/2,-y+1/2,z
y+1/2,z+1/2,x
-y+1/2,-z+1/2,x
y+1/2,-z+1/2,-x
-y+1/2,z+1/2,-x
z+1/2,x+1/2,y
-z+1/2,x+1/2,-y
-z+1/2,-x+1/2,y
z+1/2,-x+1/2,-y
y+1/2,x+1/2,z
-y+1/2,x+1/2,-z
y+1/2,-x+1/2,-z
-y+1/2,-x+1/2,z
z+1/2,y+1/2,x
-z+1/2,-y+1/2,x
-z+1/2,y+1/2,-x
z+1/2,-y+1/2,-x
x+1/2,z+1/2,y
x+1/2,-z+1/2,-y
-x+1/2,-z+1/2,y
-x+1/2,z+1/2,-y
-x+1/2,-y+1/2,-z
-x+1/2,y+1/2,z
x+1/2,-y+1/2,z
x+1/2,y+1/2,-z
-y+1/2,-z+1/2,-x
y+1/2,z+1/2,-x
-y+1/2,z+1/2,x
y+1/2,-z+1/2,x
-z+1/2,-x+1/2,-y
z+1/2,-x+1/2,y
z+1/2,x+1/2,-y
-z+1/2,x+1/2,y
-y+1/2,-x+1/2,-z
y+1/2,-x+1/2,z
-y+1/2,x+1/2,z
y+1/2,x+1/2,-z
-z+1/2,-y+1/2,-x
z+1/2,y+1/2,-x
z+1/2,-y+1/2,x
-z+1/2,y+1/2,x
-x+1/2,-z+1/2,-y
-x+1/2,z+1/2,y
x+1/2,z+1/2,-y
x+1/2,-z+1/2,y
x+1/2,y,z+1/2
x+1/2,-y,-z+1/2
-x+1/2,y,-z+1/2
-x+1/2,-y,z+1/2
y+1/2,z,x+1/2
-y+1/2,-z,x+1/2
y+1/2,-z,-x+1/2
-y+1/2,z,-x+1/2
z+1/2,x,y+1/2
-z+1/2,x,-y+1/2
-z+1/2,-x,y+1/2
z+1/2,-x,-y+1/2
y+1/2,x,z+1/2
-y+1/2,x,-z+1/2
y+1/2,-x,-z+1/2
-y+1/2,-x,z+1/2
z+1/2,y,x+1/2
-z+1/2,-y,x+1/2
-z+1/2,y,-x+1/2
z+1/2,-y,-x+1/2
x+1/2,z,y+1/2
x+1/2,-z,-y+1/2
-x+1/2,-z,y+1/2
-x+1/2,z,-y+1/2
-x+1/2,-y,-z+1/2
-x+1/2,y,z+1/2
x+1/2,-y,z+1/2
x+1/2,y,-z+1/2
-y+1/2,-z,-x+1/2
y+1/2,z,-x+1/2
-y+1/2,z,x+1/2
y+1/2,-z,x+1/2
-z+1/2,-x,-y+1/2
z+1/2,-x,y+1/2
z+1/2,x,-y+1/2
-z+1/2,x,y+1/2
-y+1/2,-x,-z+1/2
y+1/2,-x,z+1/2
-y+1/2,x,z+1/2
y+1/2,x,-z+1/2
-z+1/2,-y,-x+1/2
z+1/2,y,-x+1/2
z+1/2,-y,x+1/2
-z+1/2,y,x+1/2
-x+1/2,-z,-y+1/2
-x+1/2,z,y+1/2
x+1/2,z,-y+1/2
x+1/2,-z,y+1/2
x,y+1/2,z+1/2
x,-y+1/2,-z+1/2
-x,y+1/2,-z+1/2
-x,-y+1/2,z+1/2
y,z+1/2,x+1/2
-y,-z+1/2,x+1/2
y,-z+1/2,-x+1/2
-y,z+1/2,-x+1/2
z,x+1/2,y+1/2
-z,x+1/2,-y+1/2
-z,-x+1/2,y+1/2
z,-x+1/2,-y+1/2
y,x+1/2,z+1/2
-y,x+1/2,-z+1/2
y,-x+1/2,-z+1/2
-y,-x+1/2,z+1/2
z,y+1/2,x+1/2
-z,-y+1/2,x+1/2
-z,y+1/2,-x+1/2
z,-y+1/2,-x+1/2
x,z+1/2,y+1/2
x,-z+1/2,-y+1/2
-x,-z+1/2,y+1/2
-x,z+1/2,-y+1/2
-x,-y+1/2,-z+1/2
-x,y+1/2,z+1/2
x,-y+1/2,z+1/2
x,y+1/2,-z+1/2
-y,-z+1/2,-x+1/2
y,z+1/2,-x+1/2
-y,z+1/2,x+1/2
y,-z+1/2,x+1/2
-z,-x+1/2,-y+1/2
z,-x+1/2,y+1/2
z,x+1/2,-y+1/2
-z,x+1/2,y+1/2
-y,-x+1/2,-z+1/2
y,-x+1/2,z+1/2
-y,x+1/2,z+1/2
y,x+1/2,-z+1/2
-z,-y+1/2,-x+1/2
z,y+1/2,-x+1/2
z,-y+1/2,x+1/2
-z,y+1/2,x+1/2
-x,-z+1/2,-y+1/2
-x,z+1/2,y+1/2
x,z+1/2,-y+1/2
x,-z+1/2,y+1/2
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_type_symbol
Ce 0.00000 0.00000 0.00000 0.00619(15) 1.00000 Uiso Ce
O 0.25000 0.25000 0.25000 0.0110(8) 1.00000 Uiso O
loop_
_atom_type_symbol
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
ce 21.16710 2.81219 19.76950 0.22684 11.85130 17.60830 3.33049 127.11300
1.86264 -0.56400 2.63200
International_Tables_for_Crystallography_Vol.C(1991)_Tables_6.1.1.4_and_6.1.1.5
o 3.04850 13.27710 2.28680 5.70110 1.54630 0.32390 0.86700 32.90890 0.25080
0.00800 0.00600
International_Tables_for_Crystallography_Vol.C(1991)_Tables_6.1.1.4_and_6.1.1.5
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O Ce O 109.471(2) 1_555 2_555
O Ce O 109.471(2) 1_555 3_555
O Ce O 109.471(2) 1_555 4_555
O Ce O 180.000(3) 1_555 25_555
O Ce O 70.5288(18) 1_555 26_555
O Ce O 70.5288(18) 1_555 27_555
O Ce O 70.5288(18) 1_555 28_555
O Ce O 109.471(2) 2_555 3_555
O Ce O 109.471(2) 2_555 4_555
O Ce O 70.5288(18) 2_555 25_555
O Ce O 180.000(3) 2_555 26_555
O Ce O 70.5288(18) 2_555 27_555
O Ce O 70.5288(18) 2_555 28_555
O Ce O 109.471(2) 3_555 4_555
O Ce O 70.5288(18) 3_555 25_555
O Ce O 70.5288(18) 3_555 26_555
O Ce O 180.000(3) 3_555 27_555
O Ce O 70.5288(18) 3_555 28_555
O Ce O 70.5288(18) 4_555 25_555
O Ce O 70.5288(18) 4_555 26_555
O Ce O 70.5288(18) 4_555 27_555
O Ce O 180.000(3) 4_555 28_555
O Ce O 109.471(2) 25_555 26_555
O Ce O 109.471(2) 25_555 27_555
O Ce O 109.471(2) 25_555 28_555
O Ce O 109.471(2) 26_555 27_555
O Ce O 109.471(2) 26_555 28_555
O Ce O 109.471(2) 27_555 28_555
Ce O Ce 109.471(2) 1_555 49_555
Ce O Ce 109.471(2) 1_555 97_555
Ce O Ce 109.471(2) 1_555 145_555
Ce O O 54.7356(15) 1_555 26_555
Ce O O 125.264(3) 1_555 26_655
Ce O O 54.7356(15) 1_555 27_555
Ce O O 125.264(3) 1_555 27_565
Ce O O 54.7356(15) 1_555 28_555
Ce O O 125.264(3) 1_555 28_556
Ce O Ce 109.471(2) 49_555 97_555
Ce O Ce 109.471(2) 49_555 145_555
Ce O O 125.264(3) 49_555 26_555
Ce O O 54.7356(15) 49_555 26_655
Ce O O 125.264(3) 49_555 27_555
Ce O O 54.7356(15) 49_555 27_565
Ce O O 54.7356(15) 49_555 28_555
Ce O O 125.264(3) 49_555 28_556
Ce O Ce 109.471(2) 97_555 145_555
Ce O O 125.264(3) 97_555 26_555
Ce O O 54.7356(15) 97_555 26_655
Ce O O 54.7356(15) 97_555 27_555
Ce O O 125.264(3) 97_555 27_565
Ce O O 125.264(3) 97_555 28_555
Ce O O 54.7356(15) 97_555 28_556
Ce O O 54.7356(15) 145_555 26_555
Ce O O 125.264(3) 145_555 26_655
Ce O O 125.264(3) 145_555 27_555
Ce O O 54.7356(15) 145_555 27_565
Ce O O 125.264(3) 145_555 28_555
Ce O O 54.7356(15) 145_555 28_556
O O O 180.000(5) 26_555 26_655
O O O 90.000(2) 26_555 27_555
O O O 90.000(2) 26_555 27_565
O O O 90.000(2) 26_555 28_555
O O O 90.000(2) 26_555 28_556
O O O 90.000(2) 26_655 27_555
O O O 90.000(2) 26_655 27_565
O O O 90.000(2) 26_655 28_555
O O O 90.000(2) 26_655 28_556
O O O 180.000(5) 27_555 27_565
O O O 90.000(2) 27_555 28_555
O O O 90.000(2) 27_555 28_556
O O O 90.000(2) 27_565 28_555
O O O 90.000(2) 27_565 28_556
O O O 180.000(5) 28_555 28_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ce O 2.34248(3) 1_555
Ce O 2.34248(3) 2_555
Ce O 2.34248(3) 3_555
Ce O 2.34248(3) 4_555
Ce O 2.34248(3) 25_555
Ce O 2.34248(3) 26_555
Ce O 2.34248(3) 27_555
Ce O 2.34248(3) 28_555
O Ce 2.34248(3) 1_555
O Ce 2.34248(3) 49_555
O Ce 2.34248(3) 97_555
O Ce 2.34248(3) 145_555
O O 2.70486(6) 26_555
O O 2.70486(6) 26_655
O O 2.70486(6) 27_555
O O 2.70486(6) 27_565
O O 2.70486(6) 28_555
O O 2.70486(6) 28_556
